Journal of Materials Processing Technology 162–163 (2005) 367–372 Influence of heat treatment on the microstructure and mechanical properties of 6005 and 6082 aluminium alloys Gra˙zyna Mr´owka-Nowotnik, Jan Sieniawski ∗ Department of Materials Science, Faculty of Mechanical Engineering and Aeronautics, Rzesz´ow University of Technology, Poland Abstract The main task of this work was to study the influence of the cooling conditions after homogenization of the 6082 aluminium alloys. The effect of the solution heat treatment temperature on the mechanism and ageing kinetics of the two commercial wrought aluminum alloys 6005 and 6082 was also analyzed. The alloys were heat treated—T4 with a wide range of solution heat treatment temperature from 510 to 580 ◦ C and then natural ageing in the room temperature. Then, Brinell hardness measurements were conducted on both alloys in order to examine the influence of ageing time on the precipitation hardening behavior. The microstructure changes of the aluminium alloys following ageing for 120 h has been investigated by metallographic and transmission electron microscopy (TEM). The minor objective of the present study was to determine how extrusion processing affected the microstructure and mechanical properties of both aluminium alloys. For this purpose tensile tests were performed. © 2005 Elsevier B.V. All rights reserved. Keywords: 6xxx series Al alloys; Heat treatment; Microstructure 1. Introduction The 6xxx-group contains magnesium and silicon as major addition elements. These multiphase alloys belong to the group of commercial aluminum alloys, in which relative volume; chemical composition and morphology of structural constituents exert significant influence on their useful properties [1–5]. In the technical aluminium alloys besides the intentional additions, transition metals such as Fe and Mn are always present. Even not large amount of these impurities causes the formation of a new phase component . The exact composition of the alloy and the casting condition will directly influence the selection and volume fraction of intermetallic phases . During casting of 6xxx aluminium alloys a wide variety of Fe-containing intermetallics such as Al–Fe, Al–Fe–Si and Al–Fe–Mn–Si phases are formed between the aluminium dendrites [1–6]. Type of these phases depends mainly on the cooling rate and the Fe to Si ratio in the alloy . These intermetallic phases have different unit cell structures, morphologies, stabilities and physical and mechanical prop∗ Corresponding author. E-mail address: [email protected] (J. Sieniawski). 0924-0136/$ – see front matter © 2005 Elsevier B.V. All rights reserved. doi:10.1016/j.jmatprotec.2005.02.115 erties . As-cast billets require a homogenization treatment to make the material suitable for hot extrusion. During this homogenization treatment several processes take place such as the transformation of interconnected plate-like ␤-Al5 FeSi intermetallics into more rounded discrete ␣c -Al12 (FeMn)3 Si particles and the dissolution of ␤-Mg2 Si particles . Transformation of ␤-Al5 FeSi to ␣c -Al12 (FeMn)3 Si intermetallics is important because it improves the ductility of the material. Dissolution of ␤-Mg2 Si is also important since it will give maximum age hardening potential for the extruded product [1,3,7]. The precipitation of the metastable precursors of the equilibrium ␤-(Mg2 Si) phase occurs in one or more sequences, which are quite complex. The precipitation sequence for 6xxx alloys, which is generally accepted in the literatures [8–12], is: SSSS → atomic clusters → GP zones → ␤ → ␤ → ␤ (stable) where SSSS is the super saturated solid solution. Some authors  consider the GP zones as GP1 zones while the ␤ is called a GP2 zone. The most effective hardening phase for this types of materials is ␤ . However, the 368 Gra˙zyna Mr´owka-Nowotnik, J. Sieniawski / Journal of Materials Processing Technology 162–163 (2005) 367–372 details of changes in hardness versus annealing time and the dependence on the storage time at room temperature (RT) are not fully understood. 2. Material and experimental The investigation has been carried out on the commercial aluminum alloy – appointed in accordance with the standard PN-EN 573-3 – 6005 and 6082. The chemical composition of the alloys is indicated in Table 1. The conditions of production of the alloy were as follows: an ingot was first heated up to temperature 500 ◦ C and subsequently subjected to the extrusion forging process to obtain profiles with cross-section of a 40 mm × 100 mm. The temperature of profile going out of press was about 550 ◦ C, the cooling on exit side of the press was not applied. 2.1. Metallographic investigations The metallographic investigations of 6005 and 6082 alloy were performed on the as-cast samples, after extrusion forging process, and after natural ageing. The evolution of the microstructure of samples subjected to different cooling modes after homogenization treatment (water, oil, air and slow cooling, in the furnace) and after ageing process has been investigated. Microstructure of characteristic states of examined alloy was observed using an optical microscope – Nikon 300 and Neophot 2 on polished sections etched in Keller solution (0.5% HF in 50 ml H2 O) and transmission electron microscopy (TEM) – Tesla BS-540. 2.3. Determination of mechanical properties For determination of mechanical properties of the examined alloys, the samples were deformed in static tensile test in an Instron TTF-1115 servohydraulic universal tester at a constant rate, according to standard PN-EN 10002-1:2004. The hardness was measured with Brinell tester under 49.03 N load for 10 s. The tensile tests and hardness measurements were performed on the as-cast samples and hot-extruded samples. The hardness was also measured on the samples after homogenization treatment followed by water, oil, air and slow furnace cooling and during ageing process. 3. Results and discussion The microstructure of the studied alloys in as-cast state is given in Fig. 1a and b. In the interdendritic spaces of ␣-Al solid solution one can see the precipitates of the intermetallic phases. The revealed particles of the intermetallic phases were formed during casting of the alloy. The typical as-cast structure of examined alloys consisted of a mixture of ␤AlFeSi and ␣-AlFeMnSi intermetallic phases distributed at cell boundaries, connected sometimes with coarse Mg2 Si. 2.2. Heat treatment The temperature of homogenization treatment of 6082 alloy was determined on the basis of literature data and calorimetric investigations. The samples were preheated in an induction furnace to a temperature 570 ◦ C, held for 4 and 6 h and subsequently cooled using different cooling procedures, including a quench in water and oil, air or slow furnace cooling. Additionally, water-cooled samples were subjected to T4 heat treatment (natural ageing after solution treatment). The influence of solution heat treatment temperature on the mechanism and kinetics of ageing of the 6005 and 6082 alloys is investigated. The alloys were heat treated, with a wide range of solution heat treatment temperature from 510 to 580 ◦ C and then natural ageing in the room temperature to 120 h. In order to do the analyse of influence of time on the kinetics of ageing the Brinell hardness was measured. Table 1 Chemical composition of the investigated alloys (wt.%) Alloy Si Fe Cu Mn Mg Cr Zn Others Al 6005 6082 0.60 1.2 0.21 0.33 0.12 0.08 0.15 0.50 0.54 0.78 0.028 0.14 0.01 0.05 0.15 0.15 Bal Bal Fig. 1. Microstructure of examined as-cast alloys: (a) 6005 alloy; (b) 6082 alloy. Gra˙zyna Mr´owka-Nowotnik, J. Sieniawski / Journal of Materials Processing Technology 162–163 (2005) 367–372 369 Fig. 2. Mictostructure of examined alloys after hot extrusion: (a) 6082 alloy; (b) 6005 alloy. The microstructure of the alloy after hot extrusion forging process is given in Fig. 2a and b. During hot working of ingots, particles of intermetallic phases arrange in positions parallel to direction of plastic deformation (along plastic flow direction of processed material), which allows for the formation of the band structure. As a result, the reduction of size of larger particles may take place. Microstructures of the 6082 alloy after different modes of cooling after homogenization are shown in Fig. 3a–c. It is likely that during homogenization of the alloy at temperature 570 ◦ C, the transformation ␤-AlFeSi phase in more spheroidal ␣-Al(FeMn)Si phase may occur . It is supposed that the very fine dispersed precipitates shown in Fig. 3a–c are particles of ␤-Mg2 Si phase. The dissolved particles of ␤-Mg2 Si phase precipitates during slow cooling after homogenization . The process of natural ageing in alloy 6082 began almost instantaneously after solution heat treatment. Due to that it is not possible to observe the actual state of microstructure directly after quick cooling (in water or oil). After homogenization treatment followed by different variants of cooling the hardness of 6082 alloy was measured. The results show the considerable influence of the cooling rate after homogenizing treatment on hardness of the alloy. The highest value of hardness was obtained in the sample followed by cooling in water, however the lowest hardness Fig. 3. Microstructure of 6082 alloy after homogenization at 570 ◦ C/6 h and cooling in: (a) ice-water; (b) air and (c) in furnace. was observed for the sample cooled from the homogenization temperature in the furnace (Fig. 3c). The time of homogenization was not particularly affecting the hardness of the cooled samples (Fig. 4). The accumulation of lattice defects in the material during hot extrusion forging process exerts a considerable influence on structure formation. As a result the strain hardening of the alloy takes place and, in consequence, increases the mechanical properties. In order to compare mechanical properties of the alloy after extrusion forging process with the ones in as-cast state, the static tensile tests were performed. To confirm statistically the course of stress–strain curves, 10 370 Gra˙zyna Mr´owka-Nowotnik, J. Sieniawski / Journal of Materials Processing Technology 162–163 (2005) 367–372 Table 3 Parameters derived from Eq. (1) and hardness HB of 6082 alloy Fig. 4. Influence of different variants of cooling and of the time of homogenization on the hardness of the investigated 6082 alloy. Table 2 Mechanical properties of 6082 and 6005 Mechanical properties 6005 alloy 6082 alloy As-cast alloy Wrought alloy As-cast alloy Wrought alloy Rm (MPa) Rp0.2 (MPa) A (%) HB 120 60 17 40 155 65 21 50 130 60 25 50 170 72 25 58 separate tensile tests were done. The mechanical properties of the samples after tensile tests are shown in Table 2. One can see that, the mechanical properties of the wrought alloys are higher by about 40 MPa compared to the ones in the ascast state: the resistance Rm has grown up from the value 130 to 170 MPa for 6082 alloy and from 120 to 155 MPa for 6005 alloy (Table 2). During natural ageing of examined alloys of 6082 and 6005 the increase of hardness was observed. The ageing characteristics illustrating the changes of the hardness during ageing process of 6082 alloy are similar to that of 6005 alloy. Fig. 5 shows typical ageing curve observed for both materials after different solution heat treatment conditions. Curve in Fig. 5 shows that the hardness of the alloys increases rapidly in the initial phase of ageing, after 3 h. During following 20 h of ageing further, but insignificant increase of the hardness was observed. In order to make precise analysis of the ageing kinetics of 6005 and 6082 alloys the following equation has been used: HB = A + B ln t (1) Solution heat treatment temperature (◦ C) A B R HB 515 525 535 545 555 565 55.882 57.185 59.945 65.829 65.628 66.578 3.499 3.857 3.470 3.648 4.229 4.792 0.976 0.996 0.996 0.991 0.996 0.995 72.6 75.7 76.6 83.3 85.9 89.5 Parameters derived from the equation were presented in Tables 3 and 4. The values of regression coefficient B (Tables 3 and 4) evaluated from Eq. (1) give information about the ageing kinetics of examined alloys. Tables 3 and 4 clearly demonstrates that with regard to the 6082 alloy the ageing rate itself depends on the solution heat treatment temperature as opposed to the 6005 alloy: i.e. the higher solution treatment temperature, the higher B regression coefficient. The hardness of the 6082 alloy increase with increasing heat treatment temperature, however solutioning temperature practically does not affect the hardness of the 6005 alloy. High values of the correlation coefficient R of the 6082 alloy are evidence for strong hardness dependence on the solution heat treatment condition (temperature), nevertheless for the 6005 alloy this correlation is insignificant. The effect of the solution heat treatment condition on the hardening rate of examined alloys in form of a regression coefficient B-solutioning temperature relation illustrates Fig. 6a, 6005 alloy and Fig. 6b, 6082 alloy. The value of regression coefficient B of the 6082 alloy increases with increasing of the heat treatment temperature in accordance with the following equation: B = 0.126 exp(0.0063T ), R = 0.865 (2) i.e. the higher solution heat treatment temperature the hardening process started earliest and proceeded fastest. As shown in Fig. 6a, the kinetics of ageing of 6005 alloy does not depend on the solution heat treatment temperature. The hardness HB of the examined alloys changes similarly. During natural ageing of the 6082 alloy for 120 h, the hardness increases with rising of the solutioning temperature. It has been found that the hardness is well correlated with the solution heat treatment temperature; relationship of both parameters demonstrates a linear character and changes Table 4 Parameters derived from Eq. (1) and hardness HB of 6005 alloy Fig. 5. Exemplary ageing characteristic for both examined alloys. Solution heat treatment temperature (◦ C) A B R HB 520 530 540 550 560 570 44.706 44.073 43.615 44.481 44.449 44.184 3.030 2.924 2.732 2.935 2.878 3.092 0.982 0.970 0.989 0.983 0.984 0.991 59.214 58.072 59.474 58.534 58.228 58.989 Gra˙zyna Mr´owka-Nowotnik, J. Sieniawski / Journal of Materials Processing Technology 162–163 (2005) 367–372 371 Fig. 6. Influence of the solution heat treatment temperature on ageing kinetics of: (a) 6005 alloy; (b) 6082 alloy. in accordance with the equation: HB = 0.34T − 107.32, R = 0.985 (3) High value of the linear correlation coefficient R (Eq. (3)) is evidence for strong dependence of the solution heat treatment temperature on the hardness HB of the 6082 alloy. The hardness of the 6005 alloy the same as the ageing kinetic (Fig. 6a) does not depend on the heat treatment conditions (Fig. 7a). The lack of influence of the different treatment temperature on both the hardening velocity and the hardness of the 6005 alloy might be caused by smaller content of Mg, Si and Mn compared with (the content of these elements in) Fig. 8. Microstructure of examined alloys after ageing process: (a) 6005 alloy; (b) 6082 alloy. the 6082 alloy. It can be seen (Fig. 7b) that the hardness of 6082 alloy increases with growing of the solutioning temperature. This is due to the fact that the amount of Mg and Si in a supersaturated solution, which are essential to forming the hardening particles of ␤-Mg2 Si phase precipitated during ageing process, increases along with rising of the heat treatment temperature. The number of GP zones and strengthening phases, which are responsible for hardening of the alloys, increases with increasing of alloying components content (Fig. 8a and b). The total content of alloy forming components in the 6082 alloy come to 3.23% and it is approximately twice as much as their content in the 6005 alloy (1.808%). Hence, it can be concluded that the volume fraction of the strengthening phases in the 6005 alloy is lower which give explanation for the lack of hardening effects during natural ageing process. 4. Conclusions Fig. 7. Influence of the solution heat treatment temperature on hardness of: (a) 6005 alloy; (b) 6082 alloy. The following conclusions are drown from this work: 372 Gra˙zyna Mr´owka-Nowotnik, J. Sieniawski / Journal of Materials Processing Technology 162–163 (2005) 367–372 1. The hardness of the investigated 6082 alloy was generally more sensitive to cooling conditions then to the time of homogenization. The highest hardness was obtained in the samples cooled in water. 2. It was found that the samples after extrusion forging process show higher Rm then those in the as-cast state. 3. It was shown that the ␤-Mg2 Si phase precipitates readily during cooling after homogenization. The amount and distribution of ␤ particles depend on the cooling variant. Very fine dispersed precipitates of ␤-Mg2 Si phase were observed in the microstructure of samples cooled in air. 4. The ageing kinetics and hardness of the investigated 6005 alloy was not generally dependent on solution heat treatment temperature. Acknowledgment This work was carried out with the financial support of the Polish State Committee for Scientific Researches under Grant No. 4T08B 03222. References  N.C.W. Kuijpers, W.H. Kool, P.T.G. Koenis, K.E. Nilsen, I. Todd, S. van der Zwaag, Mater. Charact. 49 (2003) 409–420.  I.J. Polmear, Light Alloys-Metallurgy of the Light Metals, 3rd ed., Arnold, London–New York–Sydney–Auckland, London, 1995.  S. Zajac, B. Bengtsson, Ch. J¨onsson, Mater. Sci. Forum 396–402 (2002) 399–404.  M.W. Meredith, J. Worth, R.G. Hamerton, Mater. Sci. Forum 396–402 (2002) 107–112.  M. Warmuzek, J. Sieniawski, A. Gazda, G. Mr´owka, In˙z. Mat. 137 (2003) 821–824.  G. Sha, K. O’Reilly, B. Cantor, J. Worth, R. Hamerton, Mater. Sci. Eng. 304–306 (2001) 612–616.  N.C.W. Kuijpers, W.H. Kool, S. van der Zwaag, Mater. Sci. Forum 396–402 (2002) 675–680.  A.K. Gupta, D.J. Lloyd, S.A. Court, Mater. Sci. Eng. A 301 (2001) 140–146.  M. Murayama, K. Hono, M. Saga, M. Kikuchi, Mater. Sci. Eng. A 250 (1998) 127–132.  G.A. Edwards, K. Stiller, G.L. Dunlop, M.J. Couper, Acta Mater. 46 (11) (1998) 3893–3904.  C.D. Marioara, S.J. Andersen, J. Jansen, H.W. Zandbergen, Acta Mater. 49 (2001) 321–328.  W.F. Miao, D.E. Laughlin, Scripta Mater. 40 (7) (1999) 873–878.  M. Warmuzek, J. Sieniawski, A. Gazda, G. Mr´owka, Adv. Mater. Sci. 4 (2003) 81–91.
© Copyright 2019